To use all functions of this page, please activate cookies in your browser.
With an accout for my.chemeurope.com you can always see everything at a glance – and you can configure your own website and individual newsletter.
- My watch list
- My saved searches
- My saved topics
- My newsletter
Neutron diffraction is a crystallographic method for the determination of the atomic structure of a material. This is a form of elastic scattering where the neutrons exiting the experiment have more or less the same energy as the incident neutrons. The technique is similar to X-ray diffraction but the different type of radiation gives complementary information. A sample to be examined is placed in a beam of thermal or cold neutrons and the intensity pattern around the sample gives information of the structure of the material.
Additional recommended knowledge
Neutrons are particles found in the atomic nucleus of almost all atom, but they are bound. The technique requires free neutrons and these normally do not occur in nature, because they have limited life-time In a nuclear reactor, however, neutrons can be set free through nuclei decay particularly when fission occurs. All quantum particles can exhibit wave phenomena we typically associate with light or sound. Diffraction is one of these phenomena; it occurs when waves encounter obstacles whose size is comparable with the wavelength. If the wavelength of a quantum particle is short enough, atoms or their nuclei can serve as diffraction obstacles. When a beam of neutrons emanating from a reactor is slowed down and selected properly by their speed, their wavelength lies near one angstrom (0.1 nanometer), the typical separation between atoms in a solid material. Such a beam can then be used to perform a diffraction experiment. Impinging on a crystalline sample it will scatter under a limited number of well-defined angles according to the same Bragg law that describes X-ray diffraction.
A neutron diffraction measurement requires a neutron source (e.g. a nuclear reactor or spallation source), a sample (the material to be studied), and a detector. Samples sizes are relatively large compared to those used in X-ray diffraction. The technique is therefore mostly performed as powder diffraction. At a research reactor other components such as crystal monochromators or filters may be needed to select the desired neutron wavelength. Some parts of the setup may also be movable. At a spallation source the time of flight technique is used to sort the energies of the incident neutrons, so no monochromator is needed, just a bunch of electronics. (Higher energy neutrons are faster - v. simple)
Neutrons interact with matter differently than x-rays. X-rays interact primarily with the electron cloud surrounding each atom. The contribution to the diffracted x-ray intensity is therefore larger for atoms with a large atomic number (Z) than it is for atoms with a small Z. On the other hand, neutrons interact directly with the nucleus of the atom, and the contribution to the diffracted intensity is different for each isotope; for example, regular hydrogen and deuterium contribute differently. It is also often the case that light (low Z) atoms contribute strongly to the diffracted intensity even in the presence of large Z atoms. The scattering length varies from isotope to isotope rather than linearly with the atomic number. An element like Vanadium is a strong scatterer of X-rays, but its nuclei hardly scatter neutrons, which is why it often used as a container material. Non-magnetic neutron diffraction is directly sensitive to the positions of the nuclei of the atoms.
A major difference with X-rays is that the scattering is mostly due to the tiny nuclei of the atoms. That means that there is no need for a atomic form factor to describe the shape of the electron cloud of the atom and the scattering power of an atom does not fall off with the scattering angle as it does for X-rays. Diffractograms therefore can show strong well defined diffaction peaks even at high angles, particularly if the experiment is done at low temperatures. Many neutron sources are equiped with liquid Helium dewars facilitating temperatures down 4.2K. The superb high angle (i.e. high resolution) information means that the data can give very precise values for the atomic positions in the structure.
Although neutrons are uncharged, they carry a spin, and therefore interact with magnetic moments, including those arising from the electron cloud around an atom. Neutron diffraction can therefore reveal the microscopic magnetic structure of a material.
Magnetic scattering does require an atomic form factor as it is caused by the much larger electron cloud around the tiny nucleus. The intensity of the magnetic contribution to the diffraction peaks will therefore dwindle towards higher angles.
The first neutron diffraction experiments were carried out in 1945 by Ernest O. Wollan using the Graphite Reactor at Oak Ridge. He was joined shortly thereafter by Clifford Shull, and together they established the basic principles of the technique, and applied it successfully to many different materials, addressing problems like the structure of ice and the microscopic arrangements of magnetic moments in materials. For this achievement Shull was awarded one half of the 1994 Nobel Prize in Physics. Wollan had passed away in the 1990s. (The other half of the 1994 Nobel Prize for Physics went to Bert Brockhouse for development of the inelastic scattering technique at the Chalk River facility of AECL. This also involved the invention of the triple axis spectrometer). Brockhouse and Shull jointly take the somewhat dubious distinction of the longest gap between the work being done (1945) and the Nobel Prize being awarded (1994).
Neutron diffraction is closely related to X-ray powder diffraction. In fact the single crystal version of the technique is less commonly used because currently available neutron sources require relatively large samples and large single crystals are hard or impossible to come by for most materials. Future developments, however, may well change this picture. Because the data a typically a 1D powder diffractogram they are usually processed using Rietveld refinement. In fact the latter found its origin in neutron diffraction (at Petten in the Netherlands) and was later extended for use in X-ray diffraction.
Hydrogen, null-scattering and contrast variation
Neutron diffraction can be used to establish the structure of low atomic number materials like proteins and surfactants much more easily with lower flux than at a synchrotron radiation source. This is because some low atomic number materials have a higher cross section for neutron interaction than higher atomic weight materials.
One major advantage of neutron diffraction over X-ray diffraction is that the latter is rather insensitive to the presence of hydrogen in a structure, whereas the nuclei 1H and 2H=D are strong scatterers for neutrons. This means that the position of hydrogen in a crystal structure and its thermal motions can be determined far more precisely with neutrons. In addition the scattering lengths of H and D have opposite sign, which allows contrast variation. In fact there is a particular isotope ratio for which the contribution of the element would cancel, this is called null-scattering. In practice however it is not desirable to work with the relatively high concentration of H in such a sample. The scatter by H-nuclei has a large ineleastic component and this creates a large continuous background that is more or less independent of scattering angle. The elastic pattern typically consists of sharp Bragg reflections if the sample is crystalline. They tend to drown in the inelastic background. This is even more serious when the techniquw is used for the study of liquid structure. Nevertheless, by preparing samples with different isotope ratios it is possible to vary the scattering contrast enough to highlight one element in an otherwise complicated structure. The variation of other elements is possible but usually rather expensive. Hydrogen is relatively inexpensive and particularly interesting because it plays an exceptionally large role in biochemical structures and is difficult to study structurally in other ways.
|This article is licensed under the GNU Free Documentation License. It uses material from the Wikipedia article "Neutron_diffraction". A list of authors is available in Wikipedia.|